- Technical note
- Open Access
3D FEA of cemented glass fiber and cast posts with various dental cements in a maxillary central incisor
© Madfa et al. 2015
Received: 11 February 2015
Accepted: 16 September 2015
Published: 13 October 2015
This study aimed to analyse and compare the stability of two dental posts cemented with four different luting agents by examining their shear stress transfer through the FEM. Eight three-dimensional finite element models of a maxillary central incisor restored with glass fiber and Ni–Cr alloy cast dental posts. Each dental post was luted with zinc phosphate, Panavia resin, super bond C&B resin and glass ionomer materials. Finite element models were constructed and oblique loading of 100 N was applied. The distribution of shear stress was investigated at posts and cement/dentine interfaces using ABAQUS/CAE software. The peak shear stress for glass fiber post models minimized approximately three to four times of those for Ni–Cr alloy cast post models. There was negligible difference in peak of shear stress when various cements were compared, irrespective of post materials. The shear stress had same trend for all cement materials. This study found that the glass fiber dental post reduced the shear stress concentration at interfacial of post and cement/dentine compared to Ni–Cr alloy cast dental post.
Restoration of endodontically treated tooth has been greatly enhanced by many developments in materials and techniques. In many cases, the dental post is often used after root canal treatment to restore a damaged tooth with extensive loss of coronal tooth structure specifically when 50 % or massive of coronal structure have been lost (Kimmel 2000; Ferrari et al. 2001). However, the restoration of endodontically treated tooth, that including dental post, is affected by a higher risk of biomechanical failure than vital tooth (Hatzikyriakos et al. 1992). This is attributable to the relatively high fracture incidence in pulpless tooth (Salis et al. 1987) and the dental post may be displaced during function (Sorensen and Martinoff 1984). Therefore, the dental post should have enough strength to avoid fracture incidence in the remaining tooth structure and it should be cemented with sufficient bonding strength agent to prevent the dislodgment of the dental post during function (Bouillaguet et al. 2003).
Over the past years, post materials and designs have been expanded considerably to rehabilitate the endodontically treated teeth (Ferrari et al. 2000; Brown and Hicks 2002; Schwartz and Robbins 2004). In endodontics, two types of post systems, cast metal dental and prefabricated dental posts, are usually adopted to restore a root canal and provide retention for crown. Although traditional metallic cast post can be performed treatment in one dental visit, they are gradually being replaced by prefabricated posts, particularly those made with glass fiber materials (Bitter and Kielbassa 2007). The benefits for using the glass fiber dental post are aesthetics, better biocompatibility and corrosion resistance (Boschian Pest et al. 2002; Maccari et al. 2003).
Cementation of the dental post into the root canal is critical, because the process should accomplish a seal along the root canal. An ideal luting agent must meet the basic mechanical, biological and handling requisites, such as compatibility to the tooth and tissue, non-toxic, adequate working time, sufficient bonding strength, enough compressive strength, flowability, minimal microleakage, adhesiveness, ease of excess removal, low solubility in oral fluids, esthetics, and low cost (Hill 2007). However, no luting agents have all ideal properties (Creugers et al. 1994). Additionally, many studies showed conflicting in the outcomes of tensile bond strength (Creugers et al. 1994; Mendoza and Eakle 1994; Mitchell 2000). For that reason, there is no consensus in the literature as to the superiority of any cement compared to others.
Zinc phosphate cement is still the luting agent of choice for most conventional dental post restoration, because of its easy handling characteristics and long-term clinical documentation. Recently, resin-based cements were introduced and they showed good adherence to tooth structure. Many studies reported that the resin-based cements showed significantly higher retention and resistance to fatigue compared to zinc phosphate and resin-modified glass ionomer cements (Creugers et al. 1994; Mendoza and Eakle 1994; Mitchell 2000).
As the mechanical properties of the natural teeth differ from materials restoration, the interface between the components represents the critical area for stress concentration. Determination of the stress distributions in endodontically treated tooth restored with dental post is challenged owing to small dimension and complex structure of the post. However, the investigation the stress distribution in the restored endodontically treated tooth with dental post has remained controversial issue (Asmussen et al. 2005; Santos et al. 2009).
The maximum shear stress concentration at the dental post and cement/dentine interface
Ni-Cr custom-made dental post
Glass fiber dental post
The shear stress generated in endodontically restored tooth with glass fiber post was reduced approximately three to four times of those for Ni–Cr alloy cast post, when cement materials was disregarded. The maximum shear stress introduced by glass fiber post was 0.98 MPa (XY), 2 MPa (XZ) and 3 MPa (ZY). However, the maximum shear stress for Ni–Cr alloy cast post were 4.5 MPa (XY), 6 MPa (XZ) and 12 MPa (ZY). There was negligible difference in the peak of shear stresses when various cements were compared, irrespective of post materials. When post materials were disregarded, the shear stress had same trend for all cement materials.
The loss of retention for dental posts or root fracture is considered the main reason for biomechanical failure of the restoration (Bergman et al. 1989; Hatzikyriakos et al. 1992; Torbjorner et al. 1995). This study investigated the shear stress transfer at post and dentine/cement interface through the FEM. Calculated shear stresses may be compared to values of adherence obtained with resin based materials (Asmussen and Peutzfeldt 2001) or zinc phosphate cement to assess the risk of loss of retention of the dental post (Drummond et al. 1999). The higher interfacial stress concentration indicates interfacial failure of the restoration (Beer and Johnston 1993). Thus, in the present study, the shear stress was analyzed at three different plans to determine any sign, any pattern, and any location for the maximum values. The stresses analyzed under XY and XZ directions indicated that possibility of displacement of the dental post under the torsion and compression. Therefore, the use of adhesive cementation can contribute to minimize the risk of such displacement. However, stress analysis under ZY direction result in rupture of adhesive cementation at the tooth–post interface and it can therefore lead to loss of retention of the dental post. Thus, in order to increase the clinical lifespan of the restoration inside oral cavity, it is important to reduce stresses in the tooth and the post interface.
Holderegger et al. (2008) and Van Meerbeek et al. (2010) determined the bond strength of dental cements and frequently used to predict clinical behaviour of dental restorations. They reported that most annual failure rates of restorations clinically were highly correlated with the amount of shear bond strength. However, the reported bond strength values showed highly different due to the using various testing methodologies (Van Noort et al. 1989; Placido et al. 2007; Scherer et al. 2010). Additionally, the difficulty in preparing the specimens which, in turn, lead to generate non-uniform stresses within the specimens and then effect significantly on the mode of failure (Scherer et al. 2010).
To overcome these problems, FEM was used to study the shear stress distribution at the dental post and cement/dentine interface. However, accuracy and validity remain substantial challenges. In this study, accuracy was confirmed by a convergence test in which subsequent refinements of the mesh were made (Abu Kasim et al. 2011; Madfa et al. 2014). The second problem, validity, is dependent upon the extent to which the tooth model reflected the real conditions. Therefore, the models used in this study were created from a computed tomography (CT)-scan image of an adult maxillary central incisor and its surrounding structures. This provided a realistic rendition of clinical conditions. The oblique force of 100 N was obtained from the literature evaluating the mechanical behaviour of posts and cores through the FEM (Joshi et al. 2001; Asmussen et al. 2005; Al-Omiri et al. 2011; Madfa et al. 2014).
The primary role of teeth in the oral cavity is to serve as a mechanical device for the mastication of food. The stress distribution pattern in intact natural tooth is different from tooth restored with dental post system. Intact natural tooth can flex or bend during functional load while the tooth restored with dental post system showed occurrence of regions of shear stress concentration at the post and cement/dentine interfaces. This is attributable to that the post system bends or flexes as a single unit during mastication, differences of biomechanical behaviour between remaining reduced tooth structure and dental post system (Eliasson et al. 1995). Additionally, the defective in post and cement/dentine interface could cause shear stress concentration (Pegoretti et al. 2002). The results of this study were in agreement with previous studies that reported that the stress distribution were no uniform and concentrated at post and cement/dentine interfaces (Holmes et al. 1996; Alessandro et al. 2005). They reported that a very stiff post works against the natural function of the tooth creating zones of tension and shear both in the dentine and at the interfaces of the luting cement and the post.
Asmussen and Peutzfeldt (2001) reported that bonding strength of dentine bonding systems was in the range of 15–30 MPa, and posts luted with zinc phosphate cement can be displaced from its place during mastication at a stress level of approximately 5–25 MPa. In this study, the maximum shear stresses were found to be primarily located at the post and surrounding structures interface. The maximum shear stress for the fiber post models was 0.98 MPa (XY), 2 MPa (XZ) and 3 MPa (ZY). However, the maximum shear stresses for Ni–Cr alloy cast post models were 4.5 MPa (XY), 6 MPa (XZ) and 12 MPa (ZY). There was negligible difference in the peak of shear stresses when various cements were compared, irrespective of post materials. This is attributable to that the stiffness of the dental cements used in this study was near to stiffness of dentine or less.
In the current study, the Ni–Cr alloy cast post introduced higher shear stress than glass fiber post. This is due to the contact conditions and difference between the stiffness of the post, which cause amplification of stress magnitudes. These variable stress patterns suggest that increasing the modulus elasticity would increase the interfacial shear stress between the post and cement/dentine interface. The reduction in the interfacial shear stress diminishes the probability of post loosening from dentine as the stress on bonding cement is reduced. Therefore, this study recommended for practitioners utilizing glass fiber post to restore endodontically treated tooth. This is due to that the glass fiber post system can dissipate the interfacial shear stress remarkably from the coronal to the apical regions of the post.
Glass fiber post reduced the shear stress concentration at post and cement/dentine interfaces compared to Ni–Cr alloy cast post. The reduction in the interfacial shear stress for glass fiber post is advantageous as it likely to be able to resist cyclic loading and reduce the probability of root failure. Therefore, the chosen post with modulus elasticity near to the elastic properties of dentine is preferred.
There was negligible difference in the peak of shear stress when various dental cements were investigated irrespective of the post materials used. Similar trends of shear stress distribution were obtained among tested dental cements.
Solid and FE models preparation
A three-dimensional (3D) model of an adult maxillary central incisor with its surrounding cortical and cancellous bones was developed using a computed tomography (CT) scan. The 3D model was constructed along with their surrounding cortical and cancellous bones using Mimics software (Materialise NV, Belgium) and Hounsfield’s Unit. A periodontal ligament (PDL) was modelled based on the tooth root, with a thickness of 0.25 mm (Madfa et al. 2014), and it was subtracted from the volume of the cortical and cancellous bone. The restorative components of endodontically treated teeth were modelled based on the geometry of the root using a ‘Solid Works’ (Dassault Systèmes, USA). The dimension of each component was based on the data from previous studies (Pegoretti et al. 2002; Asmussen et al. 2005; Boschian Pest et al. 2006; Santos et al. 2009; Abu Kasim et al. 2011; Madfa et al. 2014).
Finite element analysis
Mechanical properties of isotropic materials
Elastic modulus (MPa)
Zinc phosphate cement
Glass ionomer cement
Superbond C&B resin cement
Mechanical properties of orthotropic materials
Glass fiber post
Glass fiber post cemented with zinc phosphate cement (FP/ZP cement).
Glass fiber post cemented with Panavia™ resin cement (FP/Panavia™ cement).
Glass fiber post cemented with superbond C&B resin cement (FP/C&B cement).
Glass fiber post cemented with glass ionomer cement (FP/GI cement).
Ni–Cr alloy cast post cemented with zinc phosphate cement (CP/ZP cement).
Ni–Cr alloy cast post cemented with Panavia™ resin cement (CP/Panavia™ cement).
Ni–Cr alloy cast post cemented with superbond C&B resin cement (CP/C&B cement).
Ni–Cr alloy cast post cemented with glass ionomer cement (CP/GI cement).
The distribution of shear stress was evaluated at the dental post and cement/dentine interfaces using ABAQUS/CAE software, Professional Version. The interfacial shear stress was calculated along the AB path from coronal to apical regions of the dental post and cement/dentine. Interfacial shear stress (τ xy , τ xz , and τ yz ) results were virtually mapped onto AB path at the post and cement/dentine interfaces. The computed interfacial stress (τ xy , τ xz , and τ yz ) results along the AB path were then analyzed.
This work was carried out in collaboration between all authors. All authors read and approved the final manuscript.
The authors wish to sincerely thank Mr. Azim Oshkour at Department of Biomedical Engineering, Faculty of Engineering, University of Malaya for his assisting in finite element modelling. This work is partly supported by the Self-Determined and Innovative Research Funds of Wuhan University of Technology (No. 2014-JL-007).
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Abu Kasim NH, Madfa AA, Hamdi M, Rahbari RG (2011) 3D-FE analysis of functionally graded structured dental posts. J Dent Mater 30:869–880View ArticleGoogle Scholar
- Alessandro L, Raffaella A, Sandro R, Davide A, Antonio A (2005) 3D FEA of cemented steel, glass and carbon posts in a maxillary incisor. Dent Mater 21:709–715View ArticleGoogle Scholar
- Al-Omiri MK, Rayyan MR, Abu-Hammad O (2011) Stress analysis of endodontically treated teeth restored with post-retained crowns: a finite element analysis study. J Am Dent Assoc 142:289–300View ArticleGoogle Scholar
- Asmussen E, Peutzfeldt A (2001) The influence of relative humidity on the effect of dentin bonding systems. J Adhes Dent 3:123–127Google Scholar
- Asmussen E, Peutzfeldt A, Sahafi A (2005) Finite element analysis of stresses in endodontically treated, dowel-restored teeth. J Prosthet Dent 94:321–329View ArticleGoogle Scholar
- Beer FP, Johnston R (1993) Transformations of stress and strain, mechanics of materials. McGraw-Hill International Editions, SingaporeGoogle Scholar
- Bergman B, Lundquist P, Sjogren U, Sundquist G (1989) Restorative and endodontic results after treatment with cast posts and cores. J Prosthet Dent 61:10–15View ArticleGoogle Scholar
- Bitter K, Kielbassa AM (2007) Post-endodontic restorations with adhesively luted fiber-reinforced composite post systems: a review. Am J Dent 20:353–360Google Scholar
- Boschian Pest L, Cavalli G, Bertani P, Gagliani M (2002) Adhesive post-endodontic restorations with fiber posts: push-out tests and SEM observations. Dent Mater 18:596–602View ArticleGoogle Scholar
- Boschian Pest L, Guidotti S, Pietrabissa R, Gagliani M (2006) Stress distribution in a post-restored tooth using the three-dimensional finite element method. J Oral Rehabil 33:690–697View ArticleGoogle Scholar
- Bouillaguet S, Troesch S, Wataha JC, Krejci I, Meyer JM, Pashley DH (2003) Microtensile bond strength between adhesive cements and root canal dentin. Dent Mater 19:199–205View ArticleGoogle Scholar
- Brown PL, Hicks NL (2003) Rehabilitation of endodontically treated teeth using the radiopaque fiber post. Compend Contin Educ Dent 24:275–278Google Scholar
- Creugers NH, Kayser AF, van’t Hof MA (1994) A meta-analysis of durability data on conventional fixed bridges. Commun Dent Oral Epidemiol 22:448–452View ArticleGoogle Scholar
- Drummond JL, Toepke TR, King TJ (1999) Thermal and cyclic loading of endodontic posts. Eur J Oral Sci 107:220–224View ArticleGoogle Scholar
- Eliasson S, Bergstrom J, Sanda A (1995) Periodontal bone loss of teeth with metal posts: a radiographic study. J Clin Periodontol 22:850–853View ArticleGoogle Scholar
- Ferrari M, Vichi A, Mannocci F, Mason PN (2000) Retrospective study of the clinical performance of fiber posts. Am J Dent 13:9B–13BGoogle Scholar
- Ferrari M, Vichi A, Grandini S, Goracci C (2001) Efficacy of a self-curing adhesive-resin cement system on luting glass-fiber posts into root canals: a SEM investigation. Int J Prosthodont 149:543–549Google Scholar
- Hatzikyriakos AH, Reisis GI, Tsingos N (1992) A 3-year postoperative clinical evaluation of posts and cores beneath existing crowns. J Prosthet Dent 67:454–458View ArticleGoogle Scholar
- Hill EE (2007) Dental cements for definitive luting: a review and practical clinical considerations. Dent Clin N Am 51:643–658View ArticleGoogle Scholar
- Holderegger C, Sailor I, Schuhmacher C, Schafer R, Hammerle C, Fischer J (2008) Shear bond strength of resin cements to human dentin. Dent Mater 24:944–950View ArticleGoogle Scholar
- Holmes DC, Diaz-Arnold AM, Leary JM (1996) Influence of post dimension on stress distribution in dentin. J Prosthet Dent 75:140–147View ArticleGoogle Scholar
- Joshi S, Mukherjee A, Kheur M, Mehta A (2001) Mechanical performance of endodontically treated teeth. Finite Elem Anal Des 37:587–601View ArticleGoogle Scholar
- Kimmel SS (2000) Restoration and reinforcement of endodontically treated teeth with a polyethylene ribbon and prefabricated fiberglass post. Gen Dent 48:700–706Google Scholar
- Maccari PC, Conceicao EN, Nunes MF (2003) Fracture resistance of endodontically treated teeth restored with three different prefabricated esthetic posts. J Esthet Restor Dent 15:25–31View ArticleGoogle Scholar
- Madfa AA, Kadir MR, Kashani J, Saidin S, Sulaiman E, Marhazlindae J, Rahbari R, Abdullah BJ, Abdullah H, Abu Kasim NH (2014) Stress distributions in maxillary central incisors restored with various types of post materials and designs. Med Eng Phys 36:962–967View ArticleGoogle Scholar
- Mendoza DB, Eakle S (1994) Retention of posts cemented with various dentinal bonding cements. J Prosthet Dent 72:591–594View ArticleGoogle Scholar
- Mitchell CA (2000) Selection of materials for post cementation. Dent Update 27:350–354Google Scholar
- Pegoretti A, Fambri L, Zappini G, Bianchetti M (2002) Finite element analysis of a glass fibre reinforced composite endodontic post. Biomaterials 23:2667–2682View ArticleGoogle Scholar
- Placido E, Mira JB, Lima RG, Muench A, de Souza RM, Ballester RY (2007) Shear versus micro-shear bond strength test: a finite element stress analysis. Dent Mater 23:1086–1092View ArticleGoogle Scholar
- Salis SG, Hood JAA, Stokes ANS, Kirk EEJ (1987) Patterns of indirect fracture in intact and restored human premolar teeth. Endod Dent Traumatol 3:10–14View ArticleGoogle Scholar
- Santos AF, Tanaka CB, Lima RG, Espósito CO, Ballester RY, Braga RR, Meira JB (2009) Vertical root fracture in upper premolars with endodontic posts: finite element analysis. J Endod 35:117–120View ArticleGoogle Scholar
- Scherer SS, Cesar PF, Swain MV (2010) Direct comparison of the bond strength results of the different test methods: a critical literature review. Dent Mater 26:e78–e93View ArticleGoogle Scholar
- Schwartz RS, Robbins JW (2004) Post placement and restoration of endodontically treated teeth: a literature review. J Endod 30:289–301View ArticleGoogle Scholar
- Sorensen JA, Martinoff JT (1984) Intracoronal reinforcement and coronal coverage: a study of endodontically treated teeth. J Prosthet Dent 51:780–784View ArticleGoogle Scholar
- Torbjorner A, Karlsson S, Odman PA (1995) Survival rate and failure characteristics for two post designs. J Prosthet Dent 73:439–444View ArticleGoogle Scholar
- Van Meerbeek B, Pumas M, Poitevin A, Mine A, Van Ende A, Neves A, De Munck J (2010) Relationship between bond-strength tests and clinical outcomes. Dent Mater 26:e100–e121View ArticleGoogle Scholar
- Van Noort R, Noose S, Howard IC, Cardew G (1989) A critique of bond strength measurements. J Dent 17:61–67View ArticleGoogle Scholar
- Yang HS, Lang LA, Guckes AD, Felton DA (2001) The effect of thermal change on various dowel-and-core restorative materials. J Prosthet Dent 86:74–80View ArticleGoogle Scholar